| ||Format||Pages||Price|| |
|7||$43.00||  ADD TO CART|
|Hardcopy (shipping and handling)||7||$43.00||  ADD TO CART|
|Standard + Redline PDF Bundle||14||$51.60||  ADD TO CART|
This test method covers the procedures for the standard practice of performing magnetic particle examination on steel forgings. The inspection medium shall consist of finely divided ferromagnetic particles, whose size, shape and magnetic properties, both individually and collectively, shall be taken into account. Forgings may be magnetized in the longitudinal or circular direction by employing the surge or continuous current flow methods. Magnetization may be applied by passing current through the piece or by inducing a magnetic field by means of a central conductor, such as a prod or yoke, or by coils. While the material is properly magnetized, the magnetic particles may be applied by either the dry method, wet method, or fluorescent method. The parts shall also be sufficiently demagnetized after inspection so that residual or leakage fields will not interfere with future operations to which the steel forgings shall be used for. Indications to be evaluated are grouped into three broad classes, namely: surface defects, which include laminar defects, forging laps and folds, flakes (thermal ruptures caused by entrapped hydrogen), heat-treating cracks, shrinkage cracks, grinding cracks, and etching or plating cracks; subsurface defects, which include stringers of nonmetallic inclusions, large nonmetallics, cracks in underbeads of welds, and forging bursts; and nonrelevant or false indications, which include magnetic writing, changes in section, edge of weld, and flow lines.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
Significance and Use
4.1 For ferromagnetic materials, magnetic particle examination is widely specified for the detection of surface and near surface discontinuities such as cracks, laps, seams, and linearly oriented nonmetallic inclusions. Such examinations are included as mandatory requirements in some forging standards such as Specification .
4.2 Use of direct current or rectified alternating (full or half wave) current as the power source for magnetic particle examination allows detection of subsurface discontinuities.
1.1 This practice covers a procedure for magnetic particle examination of steel forgings. The procedure will produce consistent results upon which acceptance standards can be based. This practice does not contain acceptance standards or recommended quality levels.
1.2 Only direct current or rectified alternating (full or half wave) current shall be used as the electric power source for any of the magnetizing methods. Alternating current is not permitted because its capability to detect subsurface discontinuities is very limited and therefore unsuitable.
1.2.1 Portable battery powered electromagnetic yokes are outside the scope of this practice.
Note 1: Guide may be utilized for magnetic particle examination in the field for machinery components originally manufactured from steel forgings.
1.3 The minimum requirements for magnetic particle examination shall conform to practice standards of Practice . If the requirements of this practice are in conflict with the requirements of Practice , the requirements of this practice shall prevail.
1.4 This practice and the applicable material specifications are expressed in both inch-pound units and SI units. However, unless the order specifies the applicable “M” specification designation [SI units], the material shall be furnished to inch-pound units.
1.5 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
1.6 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
A508/A508M Specification for Quenched and Tempered Vacuum-Treated Carbon and Alloy Steel Forgings for Pressure Vessels
E709 Guide for Magnetic Particle Testing
E1444/E1444M Practice for Magnetic Particle Testing
Other DocumentRecommendedPracticeN Supplement B-Magnetic Particle Method Available from American Society for Nondestructive Testing (ASNT), P.O. Box 28518, 1711 Arlingate Ln., Columbus, OH 43228-0518, http://www.asnt.org.
ICS Number Code 77.040.20 (Non-destructive testing of metals); 77.140.85 (Iron and steel forgings)
UNSPSC Code 31132100(Steel forgings)
ASTM A275 / A275M-15, Standard Practice for Magnetic Particle Examination of Steel Forgings, ASTM International, West Conshohocken, PA, 2015, www.astm.orgBack to Top